Solar Cells - Readings: Chapter 3

Solar Cells - Readings: Chapter 3

### Statistics

### Views

- Total Views
- 2,723
- Views on SlideShare
- 2,500
- Embed Views

### Actions

- Likes
- 1
- Downloads
- 84
- Comments
- 0

http://ocw.tudelft.nl | 220 |

https://tra.nxt-ed.com | 3 |

Solar Cells - Readings: Chapter 3

Solar Cells - Readings: Chapter 3

- Total Views
- 2,723
- Views on SlideShare
- 2,500
- Embed Views

- Likes
- 1
- Downloads
- 84
- Comments
- 0

http://ocw.tudelft.nl | 220 |

https://tra.nxt-ed.com | 3 |

- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar CellsChapter 3. SEMICONDUCTOR MATERIALS FOR SOLAR CELLS3.1 Solar cell structure In most of today solar cells the absorption of photons, which results in the generationof the charge carriers, and the subsequent separation of the photo-generated charge carrierstake place in semiconductor materials. Therefore, the semiconductor layers are the mostimportant parts of a solar cell; they form the hart of the solar cell. There are a number ofdifferent semiconductor materials that are suitable for the conversion of energy of photonsinto electrical energy, each having advantages and drawbacks. In this chapter the mostimportant semiconductor properties that determine the solar cell performance will bediscussed. The crystalline silicon (c-Si) solar cell, which dominates the PV market at present, hasa simple structure, and provides a good example of a typical solar cell structure. Figure 3.1shows the essential features of c-Si solar cells. An absorber material is typically a moderately-doped p-type square wafer having thickness around 300 µm and an area of 10 × 10 cm2 or12.5 × 12.5 cm2. On both sides of the c-Si wafer a highly doped layer is formed, n+-type onthe top side and p+-type on the back side, respectively. These highly doped layers help toseparate the photo-generated charge carriers from the bulk of the c-Si wafer. The trend in thephotovoltaic industry is to reduce the thickness of wafers up to 250 µm and to increase thearea to 20 × 20 cm2. - 3.1 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar Cells Front contact (metal grid) AR (antireflection coating) n+-type layer Serial connections to the back contact p-type of the next cell base layer p+-type layer Back contact p-n junctionFigure 3.1. A typical structure of a c-Si solar cell. In addition to semiconductor layers, solar cells consist of a top and bottom metallicgrid or another electrical contact that collects the separated charge carriers and connects thecell to a load. Usually, a thin layer that serves as an antireflective coating covers the topsideof the cell in order to decrease the reflection of light from the cell. In order to protect the cellagainst the effects of outer environment during its operation, a glass sheet or other type oftransparent encapsulant is attached to both sides of the cell. In case of thin-film solar cells,layers that constitute the cell are deposited on a substrate carrier. When the processingtemperature during the deposition of the layers is low, a wide range of low-cost substratessuch as glass sheet, metal or polymer foil can be used. The first successful solar cell was made from c-Si and c-Si is still the most widelyused PV material. Therefore we shall use c-Si as an example to explain semiconductorproperties that are relevant to solar cell operation. This gives us a basic understanding of howsolar cells based on other semiconductor materials work. The central semiconductorparameters that determine the design and performance of a solar cell are:i) concentrations of doping atoms, which can be of two different types; donor atoms which donate free electrons, ND, or acceptor atoms, which accept electrons, NA. The concentrations determine the width of a space-charge region of a junction.ii) mobility, µ, and diffusion coefficient, D, of charge carriers that characterize carriers transport due to drift and diffusion, respectively.iii) lifetime, τ, and diffusion length, L, of the excess carriers that characterize the recombination-generation processes.iv) band gap energy, EG, absorption coefficient, α, and refractive index, n, that characterize the ability of a semiconductor to absorb visible and other radiation. - 3.2 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar Cells3.2 Semiconductor properties3.2.1 Atomic structure The atomic number of Si atom is 14, it means there are 14 electrons orbiting thenucleus. In ground state configuration a Si atom has four valence electrons. These valenceelectrons are most important because they form the bonds with other Si atoms. Two Si atomsare bonded together when they share each other’s valence electron. This is the so calledcovalent bond that is formed by two electrons. Since Si atom has four valence electrons it canbe covalently bonded to four other Si atoms. In the crystalline form each Si atom is covalentlybonded to four neighbouring Si atoms. All bonds have the same length and the anglesbetween the bonds are equal. The number of bonds that an atom has with its immediateneighbours in the atomic structure is called the coordination number or coordination. Thus,in single crystal silicon, the coordination number for all Si atoms is four, we can also say thatSi atoms are fourfold coordinated. A unit cell can be defined, from which the crystal latticecan be reproduced by duplicating the unit cell and stacking the duplicates next to each other.Such a regular atomic arrangement is described as a structure with long range order. A diamond lattice unit cell represents the real lattice structure of single crystal silicon.Figure 3.2a shows the arrangement of the unit cell and Figure 3.2b the atomic structure ofsingle crystal silicon. One can determine from Figure 3.2a that there are effective eight Siatoms in the volume of the unit cell. When a lattice constant of c-Si is 5.4 Ǻ one can easilycalculate that there are approximately 5 × 1022 Si atoms per cm3. Figure 3.2 shows thecrystalline Si atomic structure with no foreign atoms. In practice, a semiconductor samplealways contains some impurity atoms. When the concentration of impurity atoms in asemiconductor is insignificant we refer to such semiconductor as an intrinsic semiconductor. At practical operational conditions, for example room temperature, there are alwayssome of the covalent bonds broken. The breaking of the bonds results in liberating the valenceelectrons from the bonds and making them mobile through the crystal lattice. We refer tothese electrons as free electrons (henceforth simply referred as electrons). The position of amissing electron in a bond, which can be regarded as positively charged, is referred to as ahole. This situation can be easily visualized by using the bonding model shown in Figure 3.3.Figure 3.2. (a) A diamond lattice unit cell representing a unit cell of single crystal Si, (b) theatomic structure of a part of single crystal Si. - 3.3 - View slide
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar Cells In the bonding model the atomic cores (atoms without valence electrons) arerepresented by circles and the valence or bonding electrons are represented by linesinterconnecting the circles. In case of c-Si one Si atom has four valence electrons and fournearest neighbours. Each of the valence electron is equally shared with the nearest neighbour.There are therefore eight lines terminating on each circle. In an ideal Si crystal at 0°K allvalence electrons take part in forming covalent bonds between Si atoms and therefore are nofree electrons in the lattice. This situation is schematically shown in Figure 3.3a. Attemperatures higher than 0°K the bonds start to break due to absorbing thermal energy. Thisprocess results in creation of mobile electrons and holes. Figure 3.3b shows a situation when acovalent bond is broken and one electron departs from the bond leaving a hole behind. Asingle line between the atoms in Figure 3.3b represents the remaining electron of the brokenbond. When a bond is broken and a hole created, a valence electron from a neighbouring bondcan “jump” into this empty position and restore the bond. The consequence of this transfer isthat at the same time the jumping electron creates an empty position in its original bond. Thesubsequent “jumps” of a valence electron can be viewed as a motion of the empty position,hole, in the direction opposite to the motion of the valence electron through the bonds. Because breaking of a covalent bond leads to the formation of an electron-hole pair, inintrinsic semiconductors the concentration of electrons is equal to the concentration of holes.At 300°K there are approximately 1.5 × 1010 broken bonds per cm3 in the intrinsic c-Si. Thisnumber then gives also the concentration of holes, p, and electrons, n, in the intrinsic c-Si. Itmeans, that at 300°K n = p = 1.5 × 1010 cm-3. This concentration is called the intrinsiccarrier concentration and is denoted ni. Si atom covalent bond electron holeFigure 3.3. The bonding model for c-Si. (a) No bonds are broken. (b) A bond between two Siatoms is broken resulting in a mobile electron and hole. - 3.4 - View slide
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar Cells3.2.2 Doping The concentrations of electrons and holes in c-Si can be manipulated by doping. Bydoping c-Si we understand that atoms of appropriate elements substitute Si atoms in thecrystal lattice. The substitution has to be carried out by atoms with three or five valenceelectrons, such as boron or phosphorous, respectively. The doping action can best beunderstood with the aid of the bonding model and is demonstrated in Figure 3.4. When introducing phosphorous atom into the c-Si lattice, four of the five phosphorousatom valence electrons will readily form bonds with the four neighbouring Si atoms. The fifthvalence electron cannot take part in forming a bond and becomes rather weakly bound to thephosphorous atom. It is easily liberated from the phosphorous atom by absorbing the thermalenergy, which is available in the c-Si lattice at room temperature. Once free, the electron canmove throughout the lattice. In this way the phosphorous atom that substitutes a Si atom inthe lattice “donates” a free (mobile) electron into the c-Si lattice. The impurity atoms thatenhance the concentration of electrons are called donors. We donate the concentration ofdonors ND. An atom with three valence electrons such as boron cannot form all bonds with fourneighbouring Si atoms when it substitutes a Si atom in the lattice. However, it can readily“accept” an electron from a nearby Si-Si bond. A thermal energy that the c-Si lattice containsat room temperature is sufficient to enable an electron from a nearby Si-Si bond to attachitself to the boron atom and complete the bonding to the four Si neighbours. In this process ahole is (a) (b) ionised P4+ atom ionised B4- atomFigure 3.4. The doping process illustrated using the bonding model. (a) A P atom substitutes aSi atom in the lattice resulting in the positively-ionised P atom and a free electron, (b) A Batom substitutes a Si atom resulting in the negatively ionised B atom and a hole. - 3.5 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar Cellscreated that can move around the lattice. The impurity atoms that enhance the concentrationof holes are called acceptors. We denote the concentration of donors NA. Note that bysubstituting Si atoms with only one type of impurity atoms, the concentration of only one typeof mobile charge carriers is increased. Charge neutrality of the material is neverthelessmaintained because the sites of the bonded and thus fixed impurity atoms become charged.The donor atoms become positively ionised and the acceptor atoms become negativelyionised. A possibility to control the electrical conductivity of a semiconductor by doping is oneof most important semiconductor features. The electrical conductivity in semiconductorsdepends on the concentration of electrons and holes and their mobility. The concentration ofelectrons and holes is influenced by the amount of the impurity atoms that are introduced intothe atomic structure of semiconductor. Figure 3.5 shows the range of doping that is used incase of c-Si. We denote a semiconductor a p-type or n-type when holes or electrons,respectively, dominate its electrical conductivity. In case that one type of charge carriers has ahigher concentration than the other type these carriers are called majority carriers (holes in thep-type and electrons in the n-type), while the other type with lower concentration are thencalled minority carriers (electrons in the p-type and holes in the n-type). Low doping Moderate doping Heavy doping 1012 1014 1016 1018 1020 Dopant concentration [cm-3]Figure 3.5. The range of doping levels used in c-Si.3.2.3 Carrier concentrations Any operation of a semiconductor device depends on the carriers that carry chargeinside the semiconductor and cause electrical currents. In order to determine and/or tounderstand device operation it is important to know the precise number of these chargecarriers. In the following section the concentrations of charge carriers inside a semiconductorare derived assuming the semiconductor is under equilibrium. The term equilibrium is used todescribe the unperturbed state of a system, to which no external voltage, magnetic field,illumination, mechanical stress, or other perturbing forces are applied. In the equilibrium statethe observable parameters of a semiconductor do not change with time. - 3.6 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar Cells In order to determine the carrier concentration one has to know the function of densityof allowed energy states of electrons and the occupation function of the allowed energy states.The density of energy states function, g(E), describes the number of allowed states per unitvolume and energy. The occupation function is the well known Fermi-Dirac distributionfunction, f(E), which describes the ratio of states filled with an electron to total allowed statesat given energy E. In an isolated Si atom, electrons are allowed to have only discrete energyvalues. The periodic atomic structure of single crystal silicon results in the ranges of allowedenergy states for electrons that are called energy bands and the excluded energy ranges,forbidden gaps or band gaps. Electrons that are liberated from the bonds determine thecharge transport in a semiconductor. Therefore, we further discuss only those bands of energylevels, which concern the valence electrons. Valence electrons, which are involved in thecovalent bonds, have their allowed energies in the valence band (VB) and the allowedenergies of electrons liberated from the covalent bonds form the conduction band (CB). Thevalence band is separated from the conduction band by a band of forbidden energy levels. Themaximum attainable valence-band energy is denoted EV, and the minimum attainableconduction-band energy is denoted EC. The energy difference between the edges of these twobands is called the band gap energy or band gap, EG, and it is an important materialparameter.EG = EC − EV (3.1) The band gap of the single crystal silicon is of 1.12 eV at room temperature. Anelectron-volt is equal to the energy, which an electron acquires when it passes through apotential of 1 volt in vacuum (1eV = 1.602 × 10-19 J). A plot of allowed electron energy statesas a function of position is called the energy band diagram and for intrinsic c-Si is shown inFigure 3.6. (a) (b) x CB E (electron energy) EC EC EG EV EV VBFigure 3.6. (a) The basic energy band diagram and (b) widely used simplified version of theenergy diagram. - 3.7 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar Cells The density of energy states at an energy E in the conduction band close to Ec and inthe valence band close to Ev are given by Eqs. (3.1). 32 ⎛ 4 2 π mn ⎞ ∗gC ( E ) = ⎜ ( E − EC ) 12 ⎜ ⎟ ⎟ (3.2a) ⎝ h3 ⎠ 32 ⎛ 4 2 π m∗ ⎞gV ( E ) = ⎜ ( E − EV ) p 12 ⎟ (3.2b) ⎜ h 3 ⎟ ⎝ ⎠ ∗where mn and m∗ is the effective mass of electrons and holes, respectively, averaged over pdifferent directions to take anisotropy into account. The Fermi-Dirac distribution function isgiven by 1f (E) = (3.3) 1 + exp ⎡( E − EF ) kT ⎤ ⎣ ⎦where k is Boltzmann’s constant (k = 1.38 × 10-23 JK-1) and EF is the so-called Fermi energy.kT is expressed in eV and equals to 0.0258 eV at 300°K. The Fermi energy is theelectrochemical potential of the electrons in a material and in this way it represents theaveraged energy of electrons in the material. The Fermi-Dirac distribution function is shownin Figure 3.7 for different temperatures. f(E) T=0°K T1>0°K T2>T1 1 0.5 0 EV EF EC EFigure 3.7. The Fermi-Dirac distribution function. For T = 0°K, all allowed states bellow theFermi level are occupied by two electrons. At T > 0°K not all states below the Fermi level areoccupied and there are some states above the Fermi level that are occupied. - 3.8 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar Cells The carriers that contribute to charge transport are electrons in the conduction bandand holes in the valence band. The total concentration of electrons in the conduction band andthe total concentration of holes in the valence band is obtained by multiplying the appropriatedensity of states function with the appropriate distribution function and integrate over thewhole energy band. Etopn=∫ gC ( E ) f ( E )dE (3.4a) EC EVp=∫ gV ( E ) ⎡1 − f ( E ) ⎤ dE ⎣ ⎦ (3.4b) EbottomSubstituting the density of states and the Fermi-Dirac distribution function into Eq. (3.4) theresulting expressions for n and p are obtained after solving the equations. The full derivationcan be found for example in reference 1.n = N C exp ⎡( EF − EC ) kT ⎤ ⎣ ⎦ for EC − EF ≥ 3kT (3.5a)p = NV exp ⎡( EV − EF ) kT ⎤ ⎣ ⎦ for EF − EV ≥ 3kT (3.5b)where NC and NV are the effective density of conduction band states and the effective densityof valence band states, respectively. In c-Si NC = 3.22 × 1019 cm-3 and NV = 1.83 × 1019 cm-3at 300°K. When the requirement that the Fermi level lies in the band gap more than 3kT fromeither band edge is satisfied the semiconductor is referred to as nondegenerate. In an intrinsic semiconductor in the equilibrium n = p = ni. When multiplying thecorresponding sides of Eqs. (3.5) one obtainsnp = ni = N C NV exp ⎣( EV − EC ) kT ⎦ = N C NV exp ⎡ − Eg kT ⎤ , 2 ⎡ ⎤ ⎣ ⎦ (3.6)which is independent of the position of the Fermi level and is valid also for dopedsemiconductors. When we denote the position of the Fermi level in the intrinsic material Eione can writeni = N C exp ⎡( Ei − EC ) kT ⎤ = NV exp ⎡( EV − Ei ) kT ⎤ ⎣ ⎦ ⎣ ⎦ (3.7)From Eq. (3.7) we can easily the position of Ei, which is given by EC + EV kT ⎛ NV ⎞ Eg kT ⎛ NV ⎞Ei = + ln ⎜ ⎟ = EC − + ln ⎜ ⎟ (3.8) 2 2 ⎝ NC ⎠ 2 2 ⎝ NC ⎠The Fermi level Ei lies close to the midgap; a slight shift is caused by the difference in theeffective densities of the valence and conduction band.1 .F. Pierret. Advanced Semiconductor Fundamentals, in Modular series on solid state devices, Vol. 6, Adison-Wesley Publishing Company, Inc., 1987. - 3.9 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar Cells It has been already mentioned in Section 3.2.2 that the concentrations of electrons andholes in c-Si can be manipulated by doping. The concentration of electrons and holes isinfluenced by the amount of the impurity atoms that substitute silicon atoms in the lattice.Under assumption that the semiconductor is uniformly doped and in equilibrium a simplerelationship between the carrier and dopant concentrations can be established. We assume thatat room temperature the dopant atoms are ionized. Inside a semiconductor the local chargedensity is given by:ρ = q ( p + ND − n − N A ) + − (3.9)where q is the elementary charge (q = 1.602 × 10-19 C). Under equilibrium conditions, in theuniformly doped semiconductor the local charge is zero, which means that the semiconductoris everywhere charge-neutral. One can write: + −p + ND − n − N A = 0 (3.10)As previously discussed, the thermal energy available at room temperature is sufficient to + +ionise almost all the dopant atoms. Under this assumption, N D ≈ N D and N A ≈ N A , oneobtainsp + ND − n − N A = 0 (3.11)which is the common form of the charge neutrality equation.Let’s consider now an n-type material. At room temperature almost all donor atoms N D areionised and donate an electron into the conduction band. Under the assumption that N A = 0 ,Eq. (3.11) becomesp + ND − n = 0 . (3.12)Under the assumption that +ND ≈ ND ≈ n (3.13)we can expect that the concentration of holes is lower than that of electrons, and becomesvery low when N D becomes very large. We can calculate more accurate the concentration ofholes in the n-type material from Eq. (3.6). ni2 ni2p= = << n (3.14) n NDIn case of a p-type material almost all acceptor atoms N A are ionised at room temperatureand accept an electron and leaving a hole in the valence band. Under the assumption that N D = 0 , Eq. (3.11) becomesp − n − NA = 0 . (3.15) - 3.10 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar CellsUnder the assumption that −NA ≈ NA ≈ p (3.16)we can expect that the concentration of electrons is lower than that of holes. We can calculatemore accurate the concentration of electrons in the p-type material from Eq. (3.6). ni2 ni2n= = << p (3.17) p NA Inserting donor and acceptor atoms into the lattice of crystalline silicon introducesallowed energy levels into the forbidden bandgap. For example, the fifth valence electron ofthe phosphorous atom does not take part in forming a bond, is rather weakly bound to theatom and easily liberates from the phosphorous atom. The energy of the liberated electron liesin the CB. The energy levels, which we denote ED, of the weakly-bound valence electrons ofthe donor atoms have to be positioned close the CB. Notice that a dashed line represents theED. This means, that an electron that occupies the ED level, is localized to the vicinity of thedonor atom. Similarly, the acceptor atoms introduce allowed energy levels EA close to the VB.Doping also influences the position of the Fermi energy. When increasing the concentrationof electrons by increasing the concentration donors the Fermi energy will increase, which isrepresented by bringing the Fermi energy close to the CB in the band diagram. In the p-typematerial the Fermi energy is moving closer the VB. A change in the Fermi-energy positionand the introduction of the allowed energy level into the bandgap due to the doping isillustrated in Figure 3.8. The position of the Fermi level in an n-type semiconductor can be calculated using Eq.(3.5a) and the assumption (3.13) and in a p-type semiconductor using Eq. (3.5b) and Eq.(3.16), respectively.EC − E F = kT ln (N C N D ) for n-type (3.18a)E F − EV = kT ln( NV N A ) for p-type (3.18b) EC EC ED EC EF EF=Ei EF EV EV EV EA intrinsic n-type p-typeFigure 3.8. A shift of the position of the Fermi energy in the band diagram and theintroduction of the allowed energy level into the bandgap due to the doping. - 3.11 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar CellsEXAMPLE.This example demonstrates how much the concentration of electrons and holes can be manipulated by doping. Ac-Si wafer is uniformly doped with 1× 1017 cm-3 phosphorous atoms. Phosphorous atoms act as donors andtherefore at room temperature the concentration of electrons is almost equal to the concentration of donoratoms: +n = N D ≈ N D = 1× 1017 cm-3.The concentration of holes in the n-type material is calculated from Eq. (3.13) ( ) 2p = ni n = 1.5 × 10 1 × 10 = 2.25× 10 cm-3. 2 10 17 3We notice that there is a difference of 14 orders between n (1× 1017 cm-3) and p (2.25 × 103 cm-3). It is nowobvious why electrons are called in the n-type material the majority carriers and holes the minority carriers. Wecan calculate the change in the Fermi energy due to the doping. Let’s assume that the reference energy level isthe bottom of the conduction band, Ec=0 eV. Using Eq. (3.8) we calculate the Fermi energy in the intrinsic c-Si.Ei = EC − EG 2 + kT 2 ln ( NV N C ) = − 1.12 2 + 0.0258 2 ln 1.83×10 ( 19 3.22×10 19 ) = − 0.57 eV .The Fermi energy in the n-type doped c-Si wafer is calculated from Eq. (3.5a)EF = EC + kT ln ( n N C ) = 0.0258 ln 1 × 10( 17 3.22 × 10 19 ) = −0.15 eV .We notice that the doping with phosphorous atoms has resulted in the shift of the Fermi energy towards the B.Note that when n > N C , the EF > EC and the Fermi energy lies in the CB. - 3.12 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar Cells3.2.4 Transport properties In contrast to the equilibrium conditions, under operational conditions a net electricalcurrent flows through a semiconductor device. The electrical currents are generated in asemiconductor due to the transport of charge from place to place by electrons and holes. Thetwo basic transport mechanisms in a semiconductor are drift and diffusion.Drift Drift is charged-particle motion in response to an electric field. In an electric field theforce acts on the charged particles in a semiconductor, which accelerates the positivelycharged holes in the direction of the electric field and the negatively charged electrons in thedirection opposite to the electric field. Because of collisions with the thermally vibratinglattice atoms and ionised impurity atoms, the carrier acceleration is frequently disturbed. Theresulting motion of electrons and holes can be described by average drift velocities vdn and vdpfor electrons and holes, respectively. In case of low electric fields, the average drift velocitiesare directly proportional to the electric field as expressed by Eqs. (3.19). The proportionalityfactor is called mobility, µ, and is a central parameter that characterises electron and holetransport due to drift.v dn = − µn ξ (3.19a)v dp = µ p ξ (3.19b)Although the electrons move in the opposite direction to the electric field, because the chargeof an electron is negative the resulting electron drift current is in the same direction as theelectric field. This is illustrated in Figure 3.9. ξ Electric field Electron flow EC JN|drift Hole flux EV JP|driftFigure 3.9. Visualization of carrier drift using the band diagram. - 3.13 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar CellsThe electron and hole drift-current densities are defined by Eqs. (3.20) and the total driftcurrent by Eq. (3.21).J N |drift = − q n v dn = q n µn ξ (3.20a)J P|drift = q p v dp = q p µ p ξ (3.20b)J drift = q ( p µ p + n µn ) ξ (3.21) Mobility is a measure of how easily the charge particles can move through asemiconductor material. For example, at 300 K, µn ≈ 1360 cm2V-1s-1 and µp ≈ 460 cm2V-1s-1 inc-Si doped with ND and NA equal to 1014 cm-3, respectively. As mentioned earlier, the motionof charged carriers is frequently disturbed by collisions. When number of collisions increases,the mobility decreases. Increasing the temperature increases the collisions of charged carrierswith the vibrating lattice atoms, which results in a lower mobility. Increasing the dopingconcentration of donors or acceptors leads to more frequent collisions with the ionised dopantatoms, which again results in a lower mobility. The dependence of mobility on doping andtemperature is in more detailed discussed in standard textbooks for semiconductor physicsand devices 1,2.Diffusion Diffusion is a process whereby particles tend to spread out from regions of highparticle concentration into regions of low particle concentration as a result of random thermalmotion. A gradient in concentration of particles in a semiconductor is the driving force for thetransport of particles associated with diffusion. On the contrary to the drift transportmechanism, the particles need not be charged to be involved in the diffusion process. Currentsresulting from diffusion are proportional to the gradient in particle concentration and areexpressed by Eqs (3.22) and the total diffusion current by Eq. (3.23). The total current due toboth drift and diffusion is expressed by Eq. (3.24).J N |diff = q DN ∇n (3.22a)J P|diff = − q DP ∇p (3.22b)J diff = q ( DN ∇n − DP ∇p ) (3.23)J = J drift + J diff = q ( p µ p + n µ n ) ξ + q ( DN ∇n − DP ∇p ) (3.24) The constants of proportionality, DN and DP, are referred to as electron and holediffusion coefficients, respectively. The diffusion coefficients of electrons and holes arelinked with the mobilities of the corresponding charge carriers by the Einstein relationship,which is expressed by Eqs. (3.25).2 D.A. Neaman, Semiconductor Physiscs and Devices: Basic principles, McGraw-Hill, 2003. - 3.14 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar CellsDN kT = (3.25a) µn qDP kT = (3.25b)µp qThe visualization of the diffusion process and the resulting directions of particle fluxes andcurrent are shown in Figure 3.10. n dn/dx>0 Electron flux EC JN|diff x p dp/dx>0 EV Hole flux JP|diff xFigure 3.10. Visualization of carrier diffusion using the band diagram.EXAMPLE. To obtain some idea about values of diffusion coefficients, let us assume Si sample at roomtemperature, doped with donors ND = 1014 cm-3. According to Eq. (3.25a)DN = ( kT q ) µ n = 0.0258 V × 1360 cm 2 V -1s -1 = 35 cm 2 s -1 . - 3.15 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar Cells3.2.5 Recombination and generation When a semiconductor is disturbed from the equilibrium state the electron and holeconcentrations change from their equilibrium values. A number of processes start within thesemiconductor after the perturbation in order to restore the equilibrium conditions. We callthese processes recombination-generation (R-G) processes and they take care that a carrierexcess or deficit is eliminated (if the perturbation is removed) or stabilized (if the perturbationis maintained). Generation is a process whereby electrons and holes are created.Recombination is a process whereby electrons and holes are annihilated or destroyed. Asmentioned earlier, several processes can occur in a semiconductor, which lead to thegeneration or annihilation of the electrons and holes. In the following we shall describe onlysome of them, which are visualized in Figure 3.11.1. Band-to-band generation (Figure 3.11a). The generation of an electron-hole pair can occur when the energy to break a bond is delivered by a photon (photogeneration) or by heat (direct thermal generation). This process can be visualized in terms of the band diagram as the excitation of an electron from the valence band into the conduction band.2. Band-to-band recombination (Figure 3.11b). This process involves the direct annihilation of a conduction-band electron with a valence-band hole and is often called direct thermal recombination. It is typically a radiative process, in which a photon is emitted that carries an excess energy released in the recombination process.3. R-G center recombination or indirect thermal recombination (Figure 3.11c). As the name suggests the annihilation or creation of electrons and holes does not occur directly but it is facilitated by a R-G center. The R-G centers can be special impurity atoms or lattice defects. Their concentration is usually small compared to the acceptor or donor concentrations. The R-G centers introduce allowed energy levels (ET) near the centre of the forbidden gap. An electron is trapped at the R-G center and consequently annihilated by a hole that is attracted by the trapped electron. Though this process seems to be less likely than the direct thermal recombination, it is at most operational conditions the dominant recombination-generation process in semiconductors. The process is typically non-radiative and the excess energy is dissipated into the lattice in form of heat. The major effect of R-G processes in a semiconductor is to produce a change in thecarrier concentration. In this way the R-G processes indirectly affects current flow insemiconductors by manipulating the concentrations of carriers that are involved in the driftand diffusion processes. The R-G processes change the carrier concentrations and this ismathematically characterized by the time rate of change in the carrier concentration (∂n/∂tand ∂p/∂t). In case of photogeneration, in which always an excess of an equal number ofelectrons and holes are created per second, one can write∂n ∂p = = GL (3.26)∂t light ∂t lightGL is the generation rate due to light and its unit is (number/cm3 s). GL is a function of thedistance in the material, depends in general on the absorption coefficient of the material,which is a function of the wavelength of light. - 3.16 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar Cells (a) EC Heat Light EV (b) EC Light (photons) EV (c) EC Heat (phonons) ET EVFigure 3.11. Visualization of some of the recombination-generation processes using thebonding model and the energy band diagram. (a) photogeneration and direct thermalgeneration, (b) direct thermal recombination, (c) R-G center (indirect thermal) recombination. We shall introduce the equations describing the rate of change in the carrierconcentration due to the dominant thermal R-G process for a semiconductor under followingcondition:(1) the semiconductor is n- or p-type and(2) the perturbation causes only low level injection.The low injection means that∆n << p0 , p ≅ p0 in a p-type material;∆p << n0 , n ≅ n0 in an n-type material. In case of the dominant thermal R-G process, which is recombination-generationinvolving R-G centres, the time rate of change in the carrier concentration depends on theexcess or deficit of electrons and holes, in respect to their equilibrium values, ∆n = n - n0 and∆p = p - p0, respectively, and the concentration of the R-G centers, NT. - 3.17 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar Cells∂n = − cn NT ∆n for electrons in a p-type material (3.27a)∂t thermal R-G∂p = − c p N T ∆p for holes in an n-type material (3.27b)∂t thermal R-Gwhere cn and cp are proportionality constants and are referred to as the electron and holecapture coefficients, respectively. The minus sign is introduced in Eqs. (3.27) because ∂n/∂tand ∂p/∂t decreases (is negative) when ∆n > 0 and ∆p > 0. We introduce the time constants 1τn = (3.28a) cn NT 1τp = (3.28b) c p NTwhich, when substituted into Eqs. (3.27), yield∂n ∆n =− for electrons in a p-type material (3.29a)∂t thermal τn R-Gdp ∆p =− for holes in an n-type material (3.29b)dt thermal τp R-G The time constants τn and τp are the central parameters associated with recombination-generation. They can be interpreted as the average time an excess minority carrier willsurvive among majority carriers. The time constants τn and τp are referred to as minority-carrier lifetimes. The values of the minority-carrier lifetimes can vary a lot. When the R-Gcenter concentration is reduced to a very low level in c-Si, a τn (τp) can achieve ~ 1 ms. On theother hand, the intentional introduction of gold atoms into Si, which introduce efficient R-Gcenters into Si, can decrease a τn (τp) to ~ 1 ns. Typical minority-carrier lifetimes in most c-Sidevices are usually ~ 1 µs. For an efficient collection of photo-generated carriers in c-Si solarcells the minority carrier lifetimes should be in range of tens of milliseconds. When an excess of generated carriers is not uniform throughout a semiconductor,diffusion of the excess carriers takes place. The excess carriers will diffuse in thesemiconductor till they do not recombine. We define the average distance that the minoritycarriers can diffuse among majority carries before being annihilated as minority-carrier-diffusion length. The minority-carrier-diffusion lengths are defined as:LN = DN τ n for electrons in a p-type material (3.30a)LP = DP τ p for holes in an n-type material (3.30b) - 3.18 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar CellsEXAMPLE. To get an idea about the diffusion lengths, let us assume room temperature, mobility of electrons ina p-type c-Si wafer to be µn ≈ 1250 cm2V-1s-1, which corresponds to doping of NA = 1014 cm-3, and τn = 10-6 s.For the given conditions, the electron diffusion length in the p-type c-Si can be calculated from Eq. (3.30a).LN = DN τ n = ( kT q ) µ n τ n = 0.02586 V × 1250 cm 2 V -1s -1 × 10 −6 s = 5.7 × 10 −3 cm = 57 µm . - 3.19 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar Cells3.2.6 Optical properties Absorption of light in a semiconductor material represents a complex interaction oflight with the semiconductor atomic structure. Only such interactions that lead to thegeneration of free charge carriers in a semiconductor, electrons and holes, contribute to thetransformation of energy carried by light into electrical energy. The generation of chargecarriers is a result of breaking of the atomic bonds, when the electron-hole pairs are created.The process of generating an electron-hole pair can be visualized in the energy band diagramas transferring an electron from the valence energy band to the conduction energy band. Thelight particles, photons, have to carry at least the energy equal to the band gap energy of asemiconductor in order to free an electron from a covalent bond. Photons with energy higherthan the band gap energy generate electron-hole pairs. Since the electrons and holes tend tooccupy energy levels at the bottom of the conduction band and the top of the valence band,respectively, the extra energy that the electron-hole pairs receive from the photons is releasedas heat into the semiconductor lattice in the thermalization process. The process of creationof an electron-hole pair by absorbing a photon and the process of thermalization areillustrated in Figure 3.12. EC EC EG Eph Eph EV EV Creation of an Thermalization electron-hole pair Eph > EGFigure 3.12. Visualization of the process of creation of an electron-hole pair by absorbing aphoton and the process of thermalization using the energy band diagram. An important key for obtaining an efficient solar cell is to minimize the heat lossesdue to the thermalization by choosing semiconductors with appropriate band gaps. Whentaking into account the energy distribution of the solar spectrum the most effective materialsfor solar energy conversion have band gap energies in the range of 1.0 to 1.8 eV (electron-volts). The photon energy, Eph, depends on the wavelength of light and is calculated using thefollowing formula:E ph = hc λ (3.31) - 3.20 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar Cellswhere h is the Planck constant (h = 6.625 × 10-34 Js) , c is the speed of light (c = 2.998 × 108ms-1), and λ is the wavelength of light. The entire spectrum of sunlight, from infrared toultraviolet, covers a range of about 0.5 eV to about 4.0 eV. About 55% of the energy ofsunlight cannot be used by most solar cells because this energy is either lower than the bandgap or it is higher and the excess energy is lost by thermalization. While the band gap energy of a semiconductor provides us with information, whichpart of the solar spectrum is absorbed, the complex refractive index, ñ = n - ik, describes howefficient the photons of a particular energy are absorbed in the material. The real part n iscalled the refractive index, and the imaginary part k is called the extinction coefficient. Theextinction coefficient is related to the absorption coefficient α by: αλk= (3.32) 4πThe n and k are called optical constants, although they are functions of the wavelength oflight or the photon energy. The wavelength, λ is related to the photon energy, hν as, hchν = (3.33) qλwhere the photon energy is represented in eV. When light impinges on an interface between two media that are characterized by theircomplex refractive indices, a part of the light is reflected from and the other part istransmitted through the interface. The interface is therefore characterized by the reflectanceand transmittance. Reflectance is the ratio of the energy reflected from the surface of theinterface to the total incident energy. Transmittance is the ratio of the energy transmittedthrough the interface to the total incident energy. When light arrives at the optical interface at normal incidence, the reflectance andtransmittance can be calculated by using the amplitude reflection and transmission ~coefficients also known as Fresnel amplitude coefficients ( ~ , t ) 3[3]: r ~ ~~ = n0 − n1r ~ ~ (3.34) n0 + n1 2n~~t = ~ 0~ (3.35) n0 + n1 ~ ~The n0 and n1 are the complex refractive indices of the first and second medium. The Fresnelamplitude coefficients are also complex numbers. The reflectance and transmittance of theinterface are:3 J.M. Bennett and H.E. Bennett, Polarization. in Handbook of Optics, eds. W.G. Driscoll and W. Vaughan,Chap. 10, Mc Graw-Hill, 1978. - 3.21 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar Cells ~ ~ 2R= r~ 2 = n0 − n1 (3.36) ~ ~ n0 + n1 ~ n ~2 4 n n ~ ~T = ~1 t = ~ 0 ~ 12 (3.37) n0 n0 + n1 When light penetrates into a material it will be absorbed as it propagates through thematerial. The absorption profile in the material depends on the absorption coefficient of thematerial, which is wavelength dependent. The most frequent approach to calculate theabsorption profile of photons in semiconductor devices is by using the Lambert-Beerabsorption formula. The Lambert-Beer formula states that a photon flux density after passinga distance x in a film with absorption coefficient α (λ ) is reduced with a factor e −α (λ ) x ,Φ( x, λ ) = Φ 0 (λ )exp(− α (λ )x ) , (3.38)where Φ 0 (λ ) is the incident photon flux density. The photon flux density is the number ofphotons per unit area per unit time and per unit wavelength. It is related to the spectral powerdensity P (λ ) associated with the solar radiation by: λΦ 0 (λ ) = P(λ ) (3.39) hcThe spectral generation rate g sp (x, λ ) , which is the number of electron-hole pairs generated ata depth x in the film per second per unit volume per unit wavelength, by photons ofwavelength λ , is calculated according to the following formula, on the assumption of zeroreflection:gsp ( x , λ ) = η g Φ 0 ( λ ) α ( λ ) e−α ( λ ) x (3.40)where ηg is the generation quantum efficiency, usually assumed to equal unity. Thisassumption means that every photon generates one and only one electron-hole pair. Theoptical generation rate GL ( x ) is calculated from the spectral generation rate by integratingover a desired wavelength spectrum: λ2GL ( x ) = ∫ g sp ( x, λ ) d λ (3.41) λ1The optical generation rate is related to the absorption profile, A(x), in the film:GL ( x ) = η g A ( x ) (3.42) λ2A ( x ) = ∫ Φ 0 ( λ ) α ( λ ) e −α ( λ ) x d λ (3.43) λ1 - 3.22 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar CellsEXAMPLE.Let’s calculate how much light is reflected from the air/c-Si interface. Lets assume that the incident light has awavelength of 500 nm. For this wavelength the complex refractive index of air is ñ0 = 1.0 –0.0 i and for c-Si ñ1= 4.293 – 0.045 i. The reflectance is calculated from Eq. 3.36. 2 2 2 n −n % % 1.0 − 0.0i − (4.293 − 0.045i ) −3.293 − 0.045iR= 0 1 = = = 0.38 . n0 + n1 % % 1.0 − 0.0i + 4.239 − 0.045i 5.293 − 0.045iIt means 38% of light with the wavelength of 500 nm is reflected from the air/c-Si interface. In case of c-Si solarcells, over 30% of the incident light in the range of interest is reflected. In order to make solar cells with a highconversion efficiency, antireflection coatings are used to reduce the reflection from c-Si solar cells.EXAMPLE.Let’s calculate the total absorption in a 300 µm thick c-Si wafer for light characterised by wavelength of 500nm. The optical constants of c-Si for light with 500 nm are: refractive index is n = 4.293, extinction coefficient k= 0.045 and absorption coefficient α = 1.11 × 104 cm-1. The incident irradiance is 1000 W/m2.First we calculate the photon flux density at 500 nm corresponding to the irradiance of 1000 W/m2. Using theEq. 3.38 we obtain (Φ 0 = P × ( λ h c ) = 1000 Wm -2 × 500 × 10−9 m / 6.625 × 10−34 Js × 2.998 × 108 ms -1 = 2.5 × 1021 m -2 s -1 . )From Eq. 3.36 we calculate how many incident photons are reflected from the surface 2 2 2 n0 − n1 % % 1.0 − 0.0i − (4.293 − 0.045i ) −3.293 − 0.045iR= = = = 0.38 n0 + n1 % % 1.0 − 0.0i + 4.239 − 0.045i 5.293 − 0.045iUsing Lambert-Beer formula (Eq. (3.38)) we calculate the photon flux density at the backside of the wafer, itmeans at the distance 300 µm from the surface. We take the reflected light into account by adapting Eq. (3.38). (Φ ( x ) = Φ 0 (1 − R ) exp ( −α x ) = 2.5 × 1021 m -2 s -1 × (1 − 0.38 ) exp −1.11 × 106 m -1 × 300 × 10-6 m ) 0The total absorption in the wafer is the difference between the photon flux density at the surface after reflectionand the photon flux density at the back of the wafer.A = ∆Φ = Φ 0 (1 − R ) − Φ ( x) = 2.5 × 1021 m -2s-1 × (1 − 0.38 ) − 0 = 1.55 × 1021 m -2s-1When we assume that all the absorbed photons generate one electron-hole pair (ηg=1), we can calculate howlarge photocurrent density corresponds to the absorbed photons.J ph = qA = 1.602 × 10−19 C × 1.55 × 1021 m -2s-1 = 248.31C m -2s -1 = 248.31 A m -2 - 3.23 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar Cells3.2.7 Carrier concentrations in non-equilibrium When a semiconductor is illuminated additional electrons and holes are generated byabsorption of photons. The photo-generated carriers interact with the semiconductor lattice.The extra energy that the electron-hole pairs receive from the photons is released into thelattice in form of heat. After this thermalization process, which is very fast and takesapproximately 10-12 s, the carrier concentrations achieve a steady-state. In this non-equilibrium state the electron and hole concentrations are different than those in theequilibrium state. In non-equilibrium states two Fermi distributions are used to describe theelectron and hole concentrations. One Fermi distribution with the quasi-Fermi energy forelectrons, EFC, describes the occupation of states in the conduction band with electrons.Another Fermi distribution with the quasi-Fermi energy for holes, EFV, describes theoccupation of states in the valence band with electrons, and therefore determines also theconcentration of holes.Using the band diagram the process of creation of electron-hole pairs and their subsequentthermalization with the quasi-Fermi levels that describe the carrier concentration underillumination is illustrated in Figure 3.13. The difference between the quasi-Fermi levels is theelectrochemical energy, µeh, of the generated electron-hole pairs which represents the measurefor the conversion efficiency of solar radiation. The density of electrons and holes under non-equilibrium conditions is described byn = N C exp[(E FC − EC ) kT ] (3.44a)p = N V exp[(EV − E FP ) kT ] (3.44b) EC EC EFC Eph µeh EFV EV EV 0s 10-12 sFigure 3.13. Thermalization photo-generated electron-hole pairs resulting in non-equilibriumcharge-carrier concentrations described by the quasi-Fermi levels. - 3.24 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar CellsIt then follows that under non-equilibrium conditions ⎡ E − EC ⎤ ⎡ E FC − E FP ⎤ ⎡ E FC − E FP ⎤n p = N C N V exp ⎢ V ⎥ exp ⎢ ⎥ = ni exp ⎢ 2 ⎥ (3.45) ⎣ kT ⎦ ⎣ kT ⎦ ⎣ kT ⎦By using the quasi-Fermi level formalism for describing the concentration of charge carriersin non-equilibrium conditions the electron and hole current densities inside a semiconductor,JN and JP, can be expressed by following equations:J N = n µ n∇EFC (3.46a)J P = p µ p∇EFV (3.46b)One can notice from Eq. (3.46) that when a quasi-Fermi level varies with position( d EFC d x ≠ 0 or d EFV d x ≠ 0 ) the current is flowing inside the semiconductor. Bychecking the position dependence of the quasi-Fermi levels in an energy band diagram, onecan easily determine whether current flows inside the semiconductor.3.3 Basic equations of device physicsIn the previous section, semiconductor material properties and the carrier transport, creationand annihilation taking place inside a semiconductor were discussed and described. Theresults from the drift, diffusion, and recombination-generation analysis are put together into aset of equations, which form a general three-dimensional mathematical model forsemiconductor device operation.3.3.1 Continuity Equations Drift, diffusion, and recombination-generation processes give rise to a change in thecarrier concentrations in time. Nevertheless, there must be a spatial and time continuity in thecarrier concentrations. The combined effect of all types of carrier action within asemiconductor is described by the following continuity equation for electrons (Eq. (3. 47a)and holes (Eq. (3.47b), respectively∂n ∂n ∂n ∂n ∂n = + + + (3.47a)∂t ∂t drift ∂t diff ∂t thermal ∂t other processes R-G (photogeneration)∂p ∂p ∂p ∂p ∂p = + + + (3.47b)∂t ∂t drift ∂t diff ∂t thermal ∂t other processes R-G (photogeneration)The continuity equations can be written in a more compact form when introducingsubstituting - 3.25 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar Cells∂n dp = − RN ; = − RP (3.48a,b)∂t thermal dt thermal R-G R-G∂n ∂p = GN ; = GP (3.49a,b)∂t other processes ∂t other processesand noting∂n ∂n 1 + = ∇ ⋅ JN (3.50a)∂t drift ∂t diff q∂p ∂p 1 + = − ∇ ⋅ JP (3.50b)∂t drift ∂t diff q In these equations ∂n/∂t (∂p/∂t) is the time rate change in the electron (hole)concentration, JN (JP) is the electron (hole) current density, RN (RP) denotes the netrecombination-generation rate of electrons (holes), GN (GP) is the generation rate of electrons(holes) due to other processes, such as photogeneration. Substituting Eqs. (3.48) through(3.50) into (3.47), we obtain∂n 1 = ∇ ⋅ J N − RN + GN (3.51a)∂t q∂p 1 = − ∇ ⋅ J P − RP + GP (3.51b)∂t q3.3.2 Current-Density Equations The electron and hole current densities inside a semiconductor, JN and JP, are obtainedby adding the current densities due to drift and diffusion.J N = q n µn ξ + q DN ∇n (3.52a)J P = q p µ p ξ − q D p ∇p (3.52b)3.3.3 Poisson’s Equation The Poisson’s equation (3.53) relates the divergence of the electric field to the spacecharge density, ρ. ρ∇ ⋅ξ = (3.53) ε rε 0 - 3.26 -
- SOLAR CELLS Chapter 3. Semiconductor Materials For Solar CellsIn this equation εr is the semiconductor dielectric constant and ε0 is the permittivity of thevacuum. The permittivity of the vacuum ε0 = 8.854x10-14 F/cm and for c-Si εr = 11.7. Freeelectrons, holes and ionised dopant atoms are the main contributors to the charge densityinside a semiconductor. It has been mentioned that impurities other than dopants and defectscan be present in a semiconductor and act as charge capture centres. However, theconcentration of such imperfections is kept small in semiconductors used for solar cells. Thespace charge density is therefore sufficiently described by Eq. (3.9):ρ = q ( p + ND − n − N A ) . + −3.3.4 Equations summary Since the operation of a solar cell can be sufficiently described by processes takingplace in one direction, the set of basic semiconductor equations will be given in one-dimensional form. dξ ρ = dx ε r ε 0 dnJ N = q n µn ξ + q DN dx dpJ P = q p µ p ξ − q DP (3.54) dx∂ n 1 dJ N = − RN + G N∂ t q dx∂p 1 dJ P =− − RP + GP∂t q dx - 3.27 -

Full NameComment goes here.MD Armanat Student 7 months ago